# Young's modulus

File:(356-365) Snapback to reality (6283432546).jpg
Rubber, a material with an extremely low Young's modulus
Young's modulus, also known as the tensile modulus or elastic modulus, is a measure of the stiffness of an elastic material and is a quantity used to characterize materials. It is defined as the ratio of the stress (force per unit area) along an axis to the strain (ratio of deformation over initial length) along that axis in the range of stress in which Hooke's law holds.

Young's modulus is the most common elastic modulus, sometimes called the modulus of elasticity, but there are other elastic moduli such as the bulk modulus and the shear modulus.

It is named after the 19th-century British scientist Thomas Young. However, the concept was developed in 1727 by Leonhard Euler, and the first experiments that used the concept of Young's modulus in its current form were performed by the Italian scientist Giordano Riccati in 1782, pre-dating Young's work by 25 years.

A material whose Young's modulus is very high is rigid. Do not confuse:

• rigidity and strength: the strength of material is characterized by its yield strength and / or its tensile strength;
• rigidity and stiffness: the beam stiffness (for example) depends on its Young's modulus but also on the ratio of its section to its length. The rigidity characterises the materials (it is an intensive property) while the stiffness regards products and constructions (it is an extensive property): a massive mechanical plastic part can be much stiffer than a steel spring;
• rigidity and hardness: the hardness of a material defines its relative resistance that its surface opposes to the penetration of a harder body.
• rigidity and toughness: toughness is the amount of energy that a material can absorb before fracturing when subjected to strain.

## Units

Young's modulus is the ratio of stress (which has units of pressure) to strain (which is dimensionless), and so Young's modulus has units of pressure. Its SI unit is therefore the pascal (Pa or N/m2 or m−1·kg·s−2). The practical units used are megapascals (MPa or N/mm2) or gigapascals (GPa or kN/mm2). In United States customary units, it is expressed as pounds (force) per square inch (psi). The abbreviation ksi refers to "kips per square inch", or thousands of psi.

## Usage

The Young's modulus enables the calculation of the change in the dimension of a bar made of an isotropic elastic material under tensile or compressive loads. For instance, it predicts how much a material sample extends under tension or shortens under compression. The Young's modulus directly applies to cases uniaxial stress, that is tensile or compressive stress in one direction and no stress in the other directions. Young's modulus is also used in order to predict the deflection that will occur in a statically determinate beam when a load is applied at a point in between the beam's supports. Other elastic calculations usually require the use of one additional elastic property, such as the shear modulus, bulk modulus or Poisson's ratio. Any two of these parameters are sufficient to fully describe elasticity in an isotropic material.

### Linear versus non-linear

The Young's modulus represents the factor of proportionality in Hooke's law, which relates the stress and the strain. However, Hooke's law is only valid under the assumption of an elastic and linear response. Any real material will eventually fail and break when stretched over a very large distance or with a very large force; however all solid materials exhibit nearly Hookean behavior for small enough strains or stresses. If the range over which Hooke's law is valid is large enough compared to the typical stress that one expects to apply to the material, the material is said to be linear. Otherwise (if the typical stress one would apply is outside the linear range) the material is said to be non-linear.

Steel, carbon fiber and glass among others are usually considered linear materials, while other materials such as rubber and soils are non-linear. However, this is not an absolute classification: if very small stresses or strains are applied to a non-linear material, the response will be linear, but if very high stress or strain is applied to a linear material, the linear theory will not be enough. For example, as the linear theory implies reversibility, it would be absurd to use the linear theory to describe the failure of a steel bridge under a high load; although steel is a linear material for most applications, it is not in such a case of catastrophic failure.

In solid mechanics, the slope of the stress–strain curve at any point is called the tangent modulus. It can be experimentally determined from the slope of a stress–strain curve created during tensile tests conducted on a sample of the material. The tangent modulus of the initial, linear portion of a stress–strain curve is called Young's modulus.

### Directional materials

Young's modulus is not always the same in all orientations of a material. Most metals and ceramics, along with many other materials, are isotropic, and their mechanical properties are the same in all orientations. However, metals and ceramics can be treated with certain impurities, and metals can be mechanically worked to make their grain structures directional. These materials then become anisotropic, and Young's modulus will change depending on the direction of the force vector. Anisotropy can be seen in many composites as well. For example, carbon fiber has much higher Young's modulus (is much stiffer) when force is loaded parallel to the fibers (along the grain). Other such materials include wood and reinforced concrete. Engineers can use this directional phenomenon to their advantage in creating structures.

## Calculation

Young's modulus, E, can be calculated by dividing the tensile stress by the extensional strain in the elastic (initial, linear) portion of the stress–strain curve:

$E \equiv \frac{\mbox {tensile stress}}{\mbox {extensional strain}} = \frac{\sigma}{\varepsilon}= \frac{F/A_0}{\Delta L/L_0} = \frac{F L_0} {A_0 \Delta L}$

where

E is the Young's modulus (modulus of elasticity)
F is the force exerted on an object under tension;
A0 is the original cross-sectional area through which the force is applied;
ΔL is the amount by which the length of the object changes;
L0 is the original length of the object.

### Force exerted by stretched or contracted material

The Young's modulus of a material can be used to calculate the force it exerts under specific strain.

$F = \frac{E A_0 \Delta L} {L_0}$

where F is the force exerted by the material when contracted or stretched by ΔL.

Hooke's law can be derived from this formula, which describes the stiffness of an ideal spring:

$F = \left( \frac{E A_0} {L_0} \right) \Delta L = k x \,$

where it comes in saturation

$k = \begin{matrix} \frac {E A_0} {L_0} \end{matrix} \,$ and $x = \Delta L. \,$

### Elastic potential energy

The elastic potential energy stored is given by the integral of this expression with respect to L:

$U_e = \int {\frac{E A_0 \Delta L} {L_0}}\, d\Delta L = \frac {E A_0} {L_0} \int { \Delta L }\, d\Delta L = \frac {E A_0 {\Delta L}^2} {2 L_0}$

where Ue is the elastic potential energy.

The elastic potential energy per unit volume is given by:

$\frac{U_e} {A_0 L_0} = \frac {E {\Delta L}^2} {2 L_0^2} = \frac {1} {2} E {\varepsilon}^2$, where $\varepsilon = \frac {\Delta L} {L_0}$ is the strain in the material.M

This formula can also be expressed as the integral of Hooke's law:

$U_e = \int {k x}\, dx = \frac {1} {2} k x^2.$

### Relation among elastic constants

For homogeneous isotropic materials simple relations exist between elastic constants (Young's modulus E, shear modulus G, bulk modulus K, and Poisson's ratio ν) that allow calculating them all as long as two are known:

$E = 2G(1+\nu) = 3K(1-2\nu).\,$

## Approximate values

File:SpiderGraph YoungMod.gif
Influences of selected glass component additions on Young's modulus of a specific base glass

Young's modulus can vary somewhat due to differences in sample composition and test method. The rate of deformation has the greatest impact on the data collected, especially in polymers. The values here are approximate and only meant for relative comparison.

Approximate Young's modulus for various materials
Material GPa psi
Rubber (small strain) 0.01–0.1 1,450–14,503
Low density polyethylene 0.11–0.86 16,000–65,000
Diatom frustules (largely silicic acid) 0.35–2.77 50,000–400,999
PTFE (Teflon) 0.5  75,000
HDPE 0.8 116,000
Bacteriophage capsids 1–3 150,000–435,000
Polypropylene 1.5–2 218,000–290,785
Polyethylene terephthalate (PET) 2–2.7 290,000–390,000
Nylon 2–4 290,000–580,000
Polystyrene 3–3.5 440,000–510,000
Medium-density fiberboard (MDF) 4 580,000
Oak wood (along grain) 11 1.60×106
Human Cortical Bone 14 2.03×106
Glass-reinforced polyester matrix  17.2 2.49×106
Aromatic peptide nanotubes  19–27 2.76×1063.92×106
High-strength concrete 30 4.35×106
Carbon fiber reinforced plastic (50/50 fibre/matrix, biaxial fabric) 30–50 4.35×1067.25×106
Hemp fiber  35 5.08×106
Magnesium metal (Mg) 45 6.53×106
Glass (see chart) 50–90 7.25×10613.1×106
Flax fiber  58 8.41×106
Aluminum 69 10.0×106
Mother-of-pearl (nacre, largely calcium carbonate)  70 10.2×106
Aramid 70.5–112.4 10.2×10616.3×106
Tooth enamel (largely calcium phosphate) 83 12.0×106
Stinging nettle fiber  87 12.6×106
Bronze 96–120 13.9×10617.4×106
Brass 100–125 14.5×10618.1×106
Titanium (Ti) 110.3 16.0×106
Titanium alloys 105–120 15.0×10617.5×106
Copper (Cu) 117 17.0×106
Carbon fiber reinforced plastic (70/30 fibre/matrix, unidirectional, along grain) 181 26.3×106
Silicon Single crystal, different directions  130–185 18.9×10626.8×106
Wrought iron 190–210 27.6×10630.5×106
Steel (ASTM-A36) 200 29.0×106
polycrystalline Yttrium iron garnet (YIG) 193 28.0×106
single-crystal Yttrium iron garnet (YIG) 200 29.0×106
Cobalt-chrome (CoCr) 220-258 29.0×106
Aromatic peptide nanospheres  230–275 33.4×10639.9×106
Beryllium (Be) 287 Script error: No such module "convert".
Molybdenum (Mo) 329 - 330    Script error: No such module "convert".
Tungsten (W) 400 – 410  Script error: No such module "convert".
Silicon carbide (SiC) 450  Script error: No such module "convert".
Tungsten carbide (WC) 450 – 650  Script error: No such module "convert".
Osmium (Os) 525 - 562  Script error: No such module "convert".
Single-walled carbon nanotube 1,000 +  Script error: No such module "convert". +
Graphene 1,050 Script error: No such module "convert".
Diamond (C) 1,050 - 1210 Script error: No such module "convert".
Carbyne (C) 32,100 Script error: No such module "convert".